Serpentinites are metamorphic rocks formed from the alteration of ultramafic rocks. These alteration processes lead to the hydration of original mineral phases that were formed prior to serpentine and other minerals [1
]. Macroscopically, foliation, which bestows a clear anisotropy to these rocks, brecciated areas, and carbonates, filling fractures or replacing serpentine minerals, are quite common features of serpentinites around the world. As a consequence of their mineralogical and structural variability, serpentinites are very heterogeneous rocks. They have been used as construction materials since ancient times; many monuments and historical buildings are made of these important heritage stones [2
]. Serpentinites appear recurrently in commercial catalogs as green marbles due to the frequent replacement of serpentine minerals for carbonates [5
]. However, they are not marbles, and a detailed characterization from several points of view (mineralogical, physical and mechanical) is needed if the rocks can be applied either in construction or conservation-restoration of the architectonic heritage.
A few published papers refer to the physical and mechanical properties of serpentinites. Coumantakis [7
] observed that in ultramaphic rocks, geomechanical behavior depends on the degree of serpentinization. Other authors [8
] report data from two construction projects in which serpentinites are used as construction material: The Hepp damn (Indonesia) and the Berke powerhouse access tunnel (Turkey). Oszoy et al. [9
] characterize serpentinites, among other stones, for the Yakakayi dam site (Turkey), highlighting their different behavior depending on the degree of alteration. Marinos et al. [10
], who also study serpentinites from the perspective of rock mass, report that the value of the Geological Index Strength (GSI) considerably differs depending on the petrographic and structural variations of serpentinites. The results of these studies have led to a common conclusion: The behavior of serpentinized rock masses depends on the degree of alteration and on the structure or foliation affecting the rock.
Other studies have approached the characterization of serpentinites without taking into account rock mass, but rather focus on the rock as dimension stone, both for conservation-restoration and new building. In this sense, Christensen [11
] describes their findings concerning the elastic properties of serpentinites and peridotites obtained from P and S wave velocities. Other authors [12
] have studied serpentinites from Egypt used as dimension stones in heritage, and Diamantis et al. [13
] have proposed several correlations among the physical and mechanical properties of Greek serpentinites used in heritage. Kurtulus et al. [14
] have determined dynamic engineering values, as well as the geotechnical and mechanical properties of serpentinized ultrabasic rocks in NW of Turkey, showing some correlations between different parameters. Navarro et al. [15
] studied the serpentinites from Macael (S of Spain) used as dimension stone, obtaining varied results with respect to their mechanical properties, owing to the mineralogical differences between samples. Other authors [16
] have compared two serpentinites from the same quarry in Macael (SE of Spain) with different degrees of carbonation. In addition, they remarked on the differences found in the main parameters used in the dimension stone industry among the samples tested. More recently, Navarro et al. [6
] have carried out a complete study with six varieties of carbonated and non-carbonated serpentinites from the SE of Spain. They showed how carbonation of serpentinites greatly influences the behavior of these rocks when used as dimension stone. Pereira et al. [5
] have remarked on the need for petrographic and mineralogical data in order to be able to decide on the utility of serpentinites as dimension stones.
A significant amount of architectonic heritage found in this part of Galicia was built using this kind of rock, which is known locally as “Pedra de Toelo” [3
]. The reason of their extensive use in the past in this area is that this stone presents the quality of being much softer and ductile to the chisel of the stonemason than the granite, another frequently used stone in the area. This characteristic allows a more refined sculpts as well as an easier finishing and polishing. Its crass shine and its color, varying from greenish to dark gray, pinkish and bluish, as well as the presence of abundant veins and a particular mottled, gives a pleasant polychrome appearance acquiring a variable tone with the changes of luminosity, originating several kinds of works. However, all these features trigger a greater degradation of the material over the passage of time [17
]. This is why most of the architectural heritage sites built on this stone are in very bad states of conservation at present, and in need of an intense conservation-restoration, including replacement of some blocks. Also for this reason, it is very important to analyze the content of asbestos in these rocks, because a high content of the fibrous minerals should prevent any intention of re-opening the quarries, to obey the very strict European laws (e.g., Directive 2009/148/EC on the protection of workers from the risks related to exposure to asbestos at work).
The quarries in this area were mined for a long period in the past centuries. In fact, they are found in the commercial catalogs under the commercial name of “Verde Pirineos” by Marmolera Gallega, S.L.; currently, a mining company is carrying out new studies and is considering the possibility of resuming mining activity. The name of the company is omitted for confidential reasons.
Preliminary studies on stones from Moeche focused on the mineralogy and the physical and mechanical characteristics of different varieties of serpentinites of the region and their use as a dimension stone in the region, which also forms part of the architectural heritage of the area [3
]. The heterogeneity of serpentinites was made clear, even within a single outcrop. The only geotechnical standard that contemplates the requirements of physical and mechanical behavior for serpentinites as natural stone is the American C1526-02 standard [21
]. In this document, the range of accepted values for water absorption (0.2% in exteriors and 0.6% in interiors) and the minimum values for uniaxial compression strength (69 MPa) and bulk density (2560 kg/m3
) are specified as the requirements.
The present paper studies the mineralogical, physical, and mechanical properties of one of the main bodies of serpentinites in Spain, located in the area surrounding Moeche (Galicia, NW of Spain). The uniaxial compression strength (UCS), elastic moduli (Es, υs), bulk density (ρ), and water absorption (a) have been determined, as well as the characterization of the mineral composition carried out using X-ray diffraction and the study of thin sections. This work also includes a detailed description of the failure surfaces developed during the UCS tests. Accordingly, ultrasonic wave velocities were measured and the results were compared to bulk density, the UCS, and the elastic moduli in search of connections that could help to explain their behavior. Furthermore, this characterization could also facilitate the commercial use of these stones, both for construction and conservation-restoration purposes.
The objectives of this work are focused on describing the main properties of serpentinites from Moeche and to determine the mechanisms of rock failure to facilitate the evaluation of these serpentinites as potential construction and conservation-restoration material.
The results obtained for the physical and mechanical properties are summarized in Table 2
Concerning the physical properties, the average bulk density was 2747 kg/m3. The highest values found corresponded to the highest values determined for VP, which were associated with sample M-7b2. The water absorption value was 0.4%, ranging between 0.1%–0.7%. One of the lowest values obtained also had a low bulk density and the lowest VP (sample M-10b), although there were no significant differences with respect to the other samples.
With regard to the mechanical properties, the uniaxial compression strengths (UCS) values were highly discordant, where the lowest value was observed for sample M-5c (24.2 MPa) and the highest for sample M-2d (119.6 MPa). The average value for the fifteen specimens tested was 57.1 MPa, the coefficient of variation, defined as the ratio of the standard deviation to the mean, being especially significant and reaching 41%. This reflects the enormous variation in the values obtained for this parameter, and the lack of meaning of averages in this context (Table 2
). Sample breakdown was reached after an axial strain between 0.07%–38% (mean 0.20%), and the Es from 12 (specimen M-10a) to 66 GPa (specimen M-7b2), with a mean of 39 GPa. Additionally, values ranged from 0.08–0.48 for the Poisson ratio, with a mean of 0.22. Most of the breakdown occurred following previous discontinuity surfaces, frequently with light colors in hand sample. The angle between the perpendicular line to the failure surface and the axis of the specimen varied between 60° and 70°.
This scattered behavior occurs quite frequently and is well known in foliated rocks [34
] as its strength is a function of the angle between the loading axis and the orientation of anisotropy planes (β). The strength is at its maximum when β is equal to 90° and at its minimum when the β angle is around 30° (45° -φ/2, being φ the friction angle of discontinuity in the Mohr-Coulomb breakdown criterion). Taking this into account, it is possible to evaluate rock anisotropy using the anisotropy ratio [37
], defined as the ratio of compressive strength at β = 90° and the minimum strength observed (σc90
). The maximum UCS obtained in the Moeche serpentinites was 119.6 MP (sample M-2d) in a nodulous serpentine with scarce planes of foliation normal to the direction of the load (β = 90°). A foliated serpentinite, on the other hand, with β = 30° and a fracture surface in a talc rich area, showed the minimum UCS (24.2 MPa, sample M-3b). This sample would be classified as high anisotropy since the ratio σc90
is between 4 and 6. Other samples with similar foliation orientations (β ≈ 30°) show a lower anisotropy ratio, which highlights that the mechanism involved in the failures also depends on the intensity of foliation, the amount of nodulous areas, and the mineralogical composition of the failure planes. Even still, the typical behavior of a foliated rock is clearly present.
According to the Reference [39
] classification for the uniaxial compression strength in rocks (Figure 3
), the samples were classified in groups that included weak to very strong rocks, with most of the samples being classified as strong (50–100 MPa). In most cases, the relative Es/UCS ratio [40
] was medium, although occasionally the ratios were high.
As for the ultrasonic velocities, VP ranged from a low of 1859 to a maximum of 5914 m/s in dried specimens. The average was 4673 m/s and the relation between the standard deviation and the average was 23%. In the case of saturated samples, the mean VP was slightly higher, 5079 m/s. The VS in dry specimens was between 1264–3342 m/s, with an average of 2627 m/s and a coefficient of variation of 21%. Under wet conditions, the average was also slightly higher: 2738 m/s. The VP/VS ratio ranged between 1.35–2.05, with a mean of 1.75.
Samples M-10a and M-10b had the lowest VP under dried conditions, obtaining values below the average, with less than 2000 m/s. Samples M-7, M-5, and M-2d displayed the highest VP values, all of them above 5000 m/s. We continue to study the correlation between ultrasonic velocities and the other parameters to understand the results, but the preliminary explanation seems to be related to the different mineralogical composition of samples, from only serpentine (antigorite) to a mixture with talc and carbonates.
The dynamic elastic modulus ranged between a minimum of 9 GPa and a maximum of 78 GPa, with a mean of 49 GPa. Evidently, the highest and the lowest values were associated with the samples with the maximum and minimum VP values.
With respect to mineralogy, the results of the x-ray diffraction (XRD) (Table 3
) showed that serpentine polymorphs (antigorite, lizardite, and traces of chrysotile) were the main minerals in all of the samples, followed by magnesite, whereas talc and dolomite appeared in smaller proportions. The latter was detected in only four samples, but these data are very important in terms of conservation-restoration, as this carbonated stone, locally called Pedra de Toelo or Pedra de Moeche, was used for the sculptures in façades of many buildings and sculptures of the region [3
] (Figure 4
Different textures were found in the Moeche serpentinites depending on the original mafic mineral and on the degree of recrystallization. In the thin sections analyzed, it was possible to distinguish the following:
Preferentially mesh texture and sometimes hour-glass texture. This is a typical texture of olivine serpentinization and is frequently observed in nodulous areas (not affected by foliation or fractures) (Figure 5
Bastite texture. Serpentine mineral aggregates elongated and with similar orientation. This is a serpentine that has replaced old pyroxenes, and in these cases, the presence of oriented magnetite following pyroxene exfoliation surfaces is quite frequent (Figure 5
Thorn texture. This has a higher degree of crystallization than the previous textures and is developed from them. Original minerals may not be clear, although there is a tendency for this texture to appear normal to olivine, and parallel to the pyroxenes (Figure 5
Fibrous serpentine (chrysotile) growing normal or parallel to fractures (Figure 5
In addition, most of the samples included chromite spinels and chromites as accessory minerals, whose borders are frequently replaced by magnetite.
The Moeche serpentinites usually showed an irregular foliation with varying directions, and wavy surfaces marked by veins filled either with carbonates or by slices parallel to them, where talc and/or serpentine was predominant. Frequent fractures running in all directions and filled with carbonates were also observed.
Foliation and fractures often affected the whole rock, but sometimes they were less persistent, leaving nodular areas with no discontinuities. These areas were of a dark green color in the hand specimens and under the petrographic microscope, serpentine, talc and carbonate could be distinguished. Some textures were the remains of the original mineralogy (olivine and pyroxene) (Figure 6
and Figure 7
In cases where a relation between rock failure and the mineralogy was established in the uniaxial compression strength test, it was observed that most of the fractures occurred following foliation or in bands parallel to this foliation. In the latter case, the predominant mineralogy was talc, a talc-serpentine association and, occasionally, carbonates filling these discontinuities. In general, the failures were not brittle, except in the case of the nodular samples, in which the fracture surface developed more irregularly and encircled porphyroblasts.
Weak specimens failed following the foliation planes defined by talc (Figure 8
a–c) or chrysotile (Figure 8
d–f), with an irregular morphology that sometimes seemed to avoid carbonated areas. This is an indication of the higher resistance present in these areas.
In moderately strong samples, the foliation was not as penetrating as in the weak samples, but was more regular (Figure 9
a–c). Unlike the weak specimens, the fractures sometimes passed through areas where carbonate recrystallization had occurred (Figure 9
Strong and very strong samples shared a brecciated aspect, but the size of the rock fragments in the strong samples was smaller (Figure 10
a,d). Also, in the strong samples, the fractures developed on foliation planes, filled with carbonate and talc (Figure 10
b,c). Moreover, when these foliation planes were not continuous, the fracture tended to surround areas containing relict porphyroblasts, usually completely serpentinized (Figure 10
Regarding the very strong samples, their fractures were brittle. It was found that neither the foliation nor the previous fracture orientations were followed, although the latter were clearly visible at the macroscopic scale, but with scarce continuity and irregular orientation (Figure 11
Moeche serpentinites show a complete transformation of primary minerals in low-grade metamorphism phases, such as minerals from serpentine, carbonate, talc and magnetite, preserving the remains of the chromium rich original spinel [41
]. All of these changes cause the mechanical properties of the rock to change, as reflected in the highly variable results obtained during the uniaxial compression strength testing carried out in this study. This parameter is significant for the determination of the behavior of dimension stones, and therefore it is important to establish the factors governing it and other properties, which can be used as an index to predict the uniaxial compression strength of these rocks.
The serpentinites of Moeche generally have low UCS, with an average value of 57 MPa, which is even below the minimum threshold required by ASTM C-1526-02 for susceptible serpentinites to be used as ornamental stones [21
]. The maximum water absorption value obtained, 0.7%, is also outside the limit values of the above standard for both outdoor (0.2%) and indoor (0.6%) use. The only ASTM requirement that these rocks accomplish is the minimum bulk density, which was 2600 kg/m3
, above the minimum value required of 2560 kg/m3
compares the properties of serpentinites from different countries reported in the literature and the ones studied here. From this data it can be observed that only the carbonated serpentinites from Macael (SE of Spain) studied by Navarro et al. [6
] fulfill all of the requirements set out by the ASTM standard (UCS > 69 MPA; ρ > 2560 kg/m3
a < 0.2% (exterior) and a < 0.6% (interior)).
The UCS values obtained are similar to the serpentinites studied in Diamantis et al. [13
] and in Kurtulus et al. [14
] from the ophiolite complex in Mount Kallidromo, in central Greece and from NW Turkey, respectively. However, differences can be found with respect to the serpentinites from Granada and Macael (SE of Spain) that have an average UCS above 227 MPa. Serpentinites can also have very high values, such as 346 MPa, as is the case of serpentinites from Granada [6
] and Egypt [12
]. But it is important to highlight that the UCS values obtained in a laboratory setting are highly dependent on multiple factors. Some of these factors are intrinsic (mineralogy, fabric or discontinuities), but others are extrinsic such as shape, size, the relation between width and length and the speed and the direction of the application of the load [42
]. UCS values obtained with different protocols (e.g., EN, ASTM) vary even with the same stone, therefore, the comparison between different stones must be approached carefully [44
]. The low resistance and significant dispersion found for this property could be explained by the macrostructure of foliated rocks such as serpentinites. The UCS in these rocks depends largely on the relative orientation between the microstructure and the axial load, and therefore the range of dispersion obtained is usually broad [40
]. This circumstance often leads to a misinterpretation of the shear strength values of discontinuity planes, where they are thought to correspond to failures in the rock matrix [10
]. There are important implications when the global behavior of serpentinized rock masses is analyzed. Upon studying several outcrops, the same authors proposed a serpentinite matrix uniaxial compression strength of around 40 MPa, which is slightly lower than the average obtained in this study (57 MPa). However, on measuring and comparing the inclinations of the principal planes of the macroscopic Moeche foliation samples tested, it was found that apparently not only the relative orientation between the load applied and the foliation control the uniaxial compression strength of these rocks (Table 5
), since there are very weak samples that, macroscopically, are not foliated, such as sample M-3b. This apparently contradicts our hypothesis, but this is in fact not the case, because under the petrographic microscope a microscopic foliation can be distinguished. Therefore, macroscopic observations alone can lead to incorrect conclusions being drawn in cases where apparently foliated specimens are analyzed, as previously noted in Hawkins et al. [28
] and references therein. By contrast, the Moeche sample M-2d is weakly foliated at both microscopic and macroscopic scale and its UCS scored the highest of all the specimens tested: 120 MPa. Therefore, as a first conclusion, it can be inferred that foliated samples are weaker than unfoliated ones. In unfoliated samples, although they are sometimes highly fractured, the presence of minerals in the fracture filling—typically carbonates—could hamper the progression of failed surfaces, resulting in a higher UCS.
In the light of the dominant role of foliation in these rocks, the question arises as to whether it might be possible that mineralogical differences between the samples could account for the wide dispersion of the UCS obtained. Figure 12
shows the mineralogy of each sample, ordered from the highest to the lowest UCS, and no clear relationship can be obtained between the UCS and the percentage of serpentine, talc, dolomite or magnesite.
Nevertheless, the relationship between the percentage of serpentine minerals and the other minerals seems to increase in the strongest samples (Figure 13
a), except for sample M-10a, which is comprised of 100% serpentine minerals but has a UCS of 36 MPa. In this sample, the orientation of the load applied and the influence of foliation prevail over mineralogy. Some authors [6
] have explained that in similar rocks the carbonate content seems to be responsible for the greater UCS. The trajectories of failure planes in weak rocks were analyzed under a petrographic microscope, and it was observed that the fractures did not progress following the path determined by carbonates. In contrast, they progressed through the carbonates in medium-strong and strong rocks (Figure 13
b). This can be explained by the alteration processes that accompany carbonation, which sometimes lead to the formation of microfractures due to the loss of material in these areas [2
]. This was also observed by Navarro et al. [6
]. In the case of carbonated serpentinites from Macael, the UCS value in the less carbonated samples was much higher than the more carbonated serpentinites. They concluded that in the initial phases of carbonation, carbonates act as cement, increasing the strength. As carbonation progresses, the pressure of crystallization produces fractures, causing the stone to become weak.
The serpentinites from Moeche vary from weak, medium strong, strong and very strong rocks, whose behavior cannot be explained only by their mineralogy. In weak samples there exists slight anisotropy defined not only by the existence of discontinuity planes, but also by a very strong preferred orientation associated with mineralogy (mainly talc); medium strong and strong samples are foliated but this feature is less intense than in the weak samples. Finally, the very strong samples display macroscopic discontinuity surfaces, but these are less continuous than in the previous cases. This fact favors a tendency towards isotropic behavior of the rock, observed microscopically in the irregular shape of the fractures formed without following any foliation or preferred mineral alignment. Glawe and Upreti [8
] classified serpentinites with discontinuities of little persistence as very strong rocks, and our data from Moeche corroborates their conclusion.
The enormous difficulties involved in obtaining samples for conducting uniaxial compression tests underscore the need for other types of much simpler tests which may provide relevant information on different mechanical aspects. The correlations between UCS and other tests or analyses are relatively abundant in the literature [45
], but they do not address serpentinites. One of the most studied correlations is bulk density and the UCS; this correlation is shown in Figure 13
c,d for the serpentinites collected from Moeche. The results are not satisfactory at all, showing a very low correlation coefficient (R2
), and disagree with the observations reported by Diamantis et al. [13
] for Greek serpentinites, Nespereira et al. [49
] for tertiary sandstones, and those of ISRM [39
]. Our results are in agreement with the data reported by Reference [50
] in sedimentary rock and Reference [51
] in basic rocks, where the relationship between the two parameters is very low. Bulk density is directly related to mineralogy, and the fact that they are not well correlated reinforces the idea that the mechanical behavior of serpentinites usually depends on several factors and is much more complex than in other types of rocks.
Other correlations considered in other works are related to the propagation velocities of ultrasonic waves. VP
correlate well with each other (Figure 14
a), but do not correlate well with the mechanical properties obtained from the uniaxial compression tests. It was apparent that the higher the VP
or the VS
, the higher the UCS, but the value of R2
ranges between 0.17–0.29 (Figure 14
b). The same can be said for the correlation between the velocities and bulk density (R2
= 0.60 to 0.59) (Figure 14
c) and between the static elastic modulus (Es
) and the velocities (Figure 13
= 0.74 to 0.72), in this case using an exponential correlation. An R2
= 0.60 is obtained for Ed
e). Comparing these results with the results for other rocks of different origin, it is common to obtain good correlations between UCS and Es
in granites, basalts and quartzites [52
], in sedimentary rocks [46
], and even in some serpentinites and peridotites [11
and UCS are also correlated positively with each other in serpentinites [13
], but much more pronounced (with R2
above 0.80 in both cases) than those observed in the Moeche rocks or in the case of serpentinites from Southern Spain, where no correlation was observed [6
]. Finally, Figure 14
e also shows the values of Es
. Their ratio lies between 1 and 2.3, with only two data points below 1. The correlation between both is similar to that obtained by Martínez-Martínez et al. [53
] for a wide range of carbonate rocks, and follows the general trend observed by Reference [54
]: As the value of Ed
increases, so does the Ed
ratio. A good correlation between VP
and Es was observed by Kurtulus et al. [14
], but in this case, the authors observed a linear correlation.
Because careful petrographic studies showed the existence of some mineral fibers in these rocks, corresponding to chrysotile, and because the increasing awareness regarding the content of asbestos in quarrying materials, we analyzed extra samples from the same quarries by SEM to clarify the major component of the serpentine phases in the rocks from Moeche. The preliminary results are compatible with all the analytical methods used to characterize the studied serpentinites: SEM shows that the major serpentine phase is antigorite (Figure 15
). A small percentage is shown as lizardite, and very few fibers of chrysotile were detected, but in a small amount that could be compatible with the potential extraction of the stone. Further studies on this subject are being carried out to study the safe handling of a potential re-opening.
Serpentinites from Moeche are very heterogeneous rocks. It is difficult to establish relatively well-defined intervals for their mechanical properties. They are rocks whose strengths range from weak to very strong, and this property seems to be reflected by the textural appearance of the rock. It is confirmed that in most cases, and in contrast to the initial general idea, the most resistant samples are those with a more brecciated aspect. This type of sample has significant carbonation that progresses, in conjunction with talc, through a network of irregular fractures, some of them coinciding with the foliation of the rock, but having poor continuity. Strongly-carbonated rocks are of interest for the potential conservation-restoration of architectural heritage that used that stone, locally named as “Pedra de Toelo” or “Pedra de Moeche”.
Continuous and persistent foliation weakens these rocks, even when detected only at a microscopic scale.
The bulk density of the Moeche serpentinites does not correlate with either the UCS or the velocity of ultrasonic waves, and hence they cannot be recommended for indirect estimations. However, ultrasonic data can be useful for obtaining a first approach to the static elastic parameters, which are usually lower than the dynamic parameters, the Ed/Es ratio increases with Ed.
The general trend observed in previous studies addressing serpentinites from other locations cannot be confirmed in the Moeche serpentinites, but, similar to the carbonated serpentinites from Macael (SE Spain), the higher the percentage of carbonates, the lower the UCS. In any case, it seems that carbonates govern the fracture morphology. What might possibly further determine the UCS in the serpentinites from Moeche is their origin; the UCS increases if there is a carbonate replacement of serpentine phases, and decreases if carbonate has filled the fractures.
A direct relationship between the mineralogical composition and the compressive strength of these rocks has not been determined. Nevertheless, a general tendency of the latter to be higher when the proportion of serpentines is also higher can be observed.
The complex relationship between mineralogy, structure, and microstructure is responsible for the large spread of values of resistance of these rocks, which in turn makes it difficult to establish a threshold value for gauging its suitability as a dimension stone based on this property. For such thresholds, these rocks do not meet American standards (ASTM), owing to their high water absorption and their low minimum UCS, which is in agreement with serpentinites from other currently operating quarries. Consequently, a draft outlining the European standards for these rocks is necessary and should include, among others, the petrographic characteristics of the rock and its mineral composition, both of which are factors that, according to the results obtained in this study, determine the geomechanical behavior of serpentinites.
According to the study presented in this paper, the serpentinites from Moeche need a complete and specific mineralogical, physical, and mechanical characterization before they can be used properly, as an ornamental stone or as conservation-restoration material, to avoid undesirable results for construction and conservation-restoration activities. Preliminary positive results associated to our research are related to the very low content of asbestos, in any of the possible phases of amphibole or chrysotile, detected in these rocks, which is an advantage is terms of quarrying even for further testing.
The present paper will be a step forward in the preservation of cultural and architectonic heritage of Galicia.